General

Property | Temperature | Value |
---|---|---|

Density | 23.0 °C | 2.7 g/cm³ Show Material materials with Density of 2.7 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Bending Fatigue Strength | 23.0 °C | 70 MPa Show Material materials with Bending Fatigue Strength of 70 MPa | |

Compressive modulus | 23.0 °C | 69.7 MPa Show Material materials with Compressive modulus of 69.7 MPa | |

Elastic modulus | 23.0 °C | 69 GPa Show Material materials with Elastic modulus of 69 GPa | |

Elongation | -195.0 °C | 28 % Show Material materials with Elongation of 28 % | Elongation in 50 mm |

-80.0 °C | 24 % Show Material materials with Elongation of 24 % | Elongation in 50 mm | |

0.0 °C | 23 % Show Material materials with Elongation of 23 % | Elongation in 50 mm | |

23.0 °C | 11 % Show Material materials with Elongation of 11 % | Elongation in 50 mm | |

24.0 °C | 22 % Show Material materials with Elongation of 22 % | Elongation in 50 mm | |

100.0 °C | 18 % Show Material materials with Elongation of 18 % | Elongation in 50 mm | |

150.0 °C | 20 % Show Material materials with Elongation of 20 % | Elongation in 50 mm | |

205.0 °C | 40 % Show Material materials with Elongation of 40 % | Elongation in 50 mm | |

260.0 °C | 75 % Show Material materials with Elongation of 75 % | Elongation in 50 mm | |

315.0 °C | 80 % Show Material materials with Elongation of 80 % | Elongation in 50 mm | |

370.0 °C | 105 % Show Material materials with Elongation of 105 % | Elongation in 50 mm | |

Elongation A100 | 23.0 °C | 7 % Show Material materials with Elongation A100 of 7 % | |

Elongation A50 | 23.0 °C | 8 - 12 % Show Material materials with Elongation A50 of 8 - 12 % | |

Fatigue strength | 23.0 °C | 69 MPa Show Material materials with Fatigue strength of 69 MPa | fo 5x10⁸ cycles |

Hardness, Brinell | 23.0 °C | 60 [-] Show Material materials with Hardness, Brinell of 60 [-] | 500 kg load, 10 mm ball |

Plane-Strain Fracture Toughnes | 23.0 °C | 22 - 35 MPa·√m Show Material materials with Plane-Strain Fracture Toughnes of 22 - 35 MPa·√m | Typical for Wrought 6000 Series Aluminium |

Poisson's ratio | 23.0 °C | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | Typical for Wrought 6000 Series Aluminium |

Shear modulus | 23.0 °C | 26 - 26.5 GPa Show Material materials with Shear modulus of 26 - 26.5 GPa | Typical for Wrought 6000 Series Aluminium |

Shear strength | 23.0 °C | 117 MPa Show Material materials with Shear strength of 117 MPa | |

Tensile strength | -195.0 °C | 255 MPa Show Material materials with Tensile strength of 255 MPa | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture |

-80.0 °C | 200 MPa Show Material materials with Tensile strength of 200 MPa | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | |

0.0 °C | 193 MPa Show Material materials with Tensile strength of 193 MPa | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | |

23.0 °C | 145 - 185 MPa Show Material materials with Tensile strength of 145 - 185 MPa | ||

24.0 °C | 185 MPa Show Material materials with Tensile strength of 185 MPa | ||

100.0 °C | 165 MPa Show Material materials with Tensile strength of 165 MPa | ||

150.0 °C | 138 MPa Show Material materials with Tensile strength of 138 MPa | ||

205.0 °C | 62 MPa Show Material materials with Tensile strength of 62 MPa | ||

260.0 °C | 31 MPa Show Material materials with Tensile strength of 31 MPa | ||

315.0 °C | 22 MPa Show Material materials with Tensile strength of 22 MPa | ||

370.0 °C | 16 MPa Show Material materials with Tensile strength of 16 MPa | ||

Unlock all property charts | |||

Yield strength | 23.0 °C | 140 MPa Show Material materials with Yield strength of 140 MPa | |

Yield strength Rp0.2 | -196.0 °C | 165 MPa Show Material materials with Yield strength Rp0.2 of 165 MPa | |

-80.0 °C | 152 MPa Show Material materials with Yield strength Rp0.2 of 152 MPa | ||

-28.0 °C | 152 MPa Show Material materials with Yield strength Rp0.2 of 152 MPa | ||

23.0 °C | 105 - 145 MPa Show Material materials with Yield strength Rp0.2 of 105 - 145 MPa | ||

24.0 °C | 145 MPa Show Material materials with Yield strength Rp0.2 of 145 MPa | ||

100.0 °C | 138 MPa Show Material materials with Yield strength Rp0.2 of 138 MPa | ||

149.0 °C | 124 MPa Show Material materials with Yield strength Rp0.2 of 124 MPa | ||

204.0 °C | 45 MPa Show Material materials with Yield strength Rp0.2 of 45 MPa | ||

260.0 °C | 24 MPa Show Material materials with Yield strength Rp0.2 of 24 MPa | ||

316.0 °C | 17 MPa Show Material materials with Yield strength Rp0.2 of 17 MPa | ||

371.0 °C | 14 MPa Show Material materials with Yield strength Rp0.2 of 14 MPa | ||

Unlock all property charts |

Thermal

Property | Temperature | Value |
---|---|---|

Coefficient of thermal expansion | 20.0 °C | 2.34E-5 1/K Show Material materials with Coefficient of thermal expansion of 2.34E-5 1/K |

23.0 °C | 2.3E-5 1/K Show Material materials with Coefficient of thermal expansion of 2.3E-5 1/K | |

100.0 °C | 2.34E-5 1/K Show Material materials with Coefficient of thermal expansion of 2.34E-5 1/K | |

Unlock all property charts | ||

Melting point | 615 - 655 °C Show Material materials with Melting point of 615 - 655 °C | |

Specific heat capacity | 23.0 °C | 900 J/(kg·K) Show Material materials with Specific heat capacity of 900 J/(kg·K) |

Thermal conductivity | 23.0 °C | 193 - 218 W/(m·K) Show Material materials with Thermal conductivity of 193 - 218 W/(m·K) |

Electrical

Property | Temperature | Value | Comment |
---|---|---|---|

Electrical conductivity | 23.0 °C | 2.90E+7 - 3.40E+7 S/m Show Material materials with Electrical conductivity of 2.90E+7 - 3.40E+7 S/m | Typical value |

Electrical resistivity | 23.0 °C | 2.94E-8 - 3.45E-8 Ω·m Show Material materials with Electrical resistivity of 2.94E-8 - 3.45E-8 Ω·m | Typical value |

Specific Electrical conductivity | 55 % IACS Show Material materials with Specific Electrical conductivity of 55 % IACS | Typical/Derived value |

Chemical properties

Property | Value | Comment |
---|---|---|

Aluminium | 97.5 - 99.4 % Show Material materials with Aluminium of 97.5 - 99.4 % | |

Chromium | 0 - 0.1 % Show Material materials with Chromium of 0 - 0.1 % | |

Copper | 0 - 0.1 % Show Material materials with Copper of 0 - 0.1 % | |

Iron | 0 - 0.35 % Show Material materials with Iron of 0 - 0.35 % | |

Magnesium | 0.45 - 0.9 % Show Material materials with Magnesium of 0.45 - 0.9 % | |

Manganese | 0 - 0.1 % Show Material materials with Manganese of 0 - 0.1 % | |

Other | 0 - 0.15 % Show Material materials with Other of 0 - 0.15 % | each 0.05, total 0.15, Rest Al |

Silicon | 0.2 - 0.6 % Show Material materials with Silicon of 0.2 - 0.6 % | |

Titanium | 0 - 0.1 % Show Material materials with Titanium of 0 - 0.1 % | |

Zinc | 0 - 0.1 % Show Material materials with Zinc of 0 - 0.1 % |

Technological properties

Property | ||
---|---|---|

Brazing | general: possible with commercial processes and methods | |

Corrosion properties | Stress corrosion cracking: no damage during operation and laboratory tests, general: very good, without protection in industrial or seawater atmosphere | |

General machinability | General: poor (T1, T4), sufficient (T5, T452, T6, T83, T831, T832) | |

Workability | general (condition): acceptable (T1, T4, T5, T452), poor(T6, T83, T831, T832) |